Assuring Quality of Masonry Mortar
LEARNING OBJECTIVES n
Understand the ASTM standards pertaining to masonry mortar. Understand the correct mortar types for various types of masonry construction. Understand the various materials for mortar. Understand the Quality Assurance options for mortar. Understand methods to ensure a consistent mortar appearance.
ASTM Standards ASTM C270 - Specification for Mortar for Unit Masonry ASTM C780 – Test Method for Preconstruction and Construction Evaluation of Mortars for Plain and Reinforced Unit Masonry ASTM C1471 – Specification for Preblended Dry Mortar Mix for Unit Masonry ASTM C1586 - Guide for Mortar for Unit Masonry
Guide for Quality Assurance of Mortars ASTM C1586
ASTM C 1586
Specification for Mortar for Unit Masonry ASTM C270
ASTM C 270
Steps in Specifying Mortar Step 1. Determine Mortar Type Step 2. Determine Mortar Materials Step 3. Determine Mortar Specification Step 4. Determine Mix Proportions Step 5. Specify a QA Procedure
Step 1 Determine Mortar Type
1. Determine Mortar Type M . . . . . . . .2500 psi A S . . .. . . . . . . 1800 psi O N . . . . . . . . . . 750 psi W O . . . . . . . . . . 350 psi R K . . . . . . . . . . . 75 psi(?)
1. Determine Mortar Type Mortar Type Recommended Alternative
load-bearing wall non-load bearing wall parapet wall
N O N
S or M N or S S
foundation wall, retaining wall, manholes, sewers, pavements, walks & patios
M or N
load-bearing wall non-bearing partitions
S or M N
1. Determine Mortar Type 5. Requirements
Bond is more important. 0.44
Prism (wall) Compressive Strength (psi)
”5.1 … A mortar type of known higher strength shall not be indiscriminately substituted where a mortar type of anticipated lower strength is specified.” 1750 1700 1650 1600 1550 1500
Mortar increase = 100% Wall increase = 7%
1450 1400 0
Mortar Compressive Strength (psi)
Step 2 Determine Mortar Materials
2. Determine Mortar Materials n n n n n n n n
Portland Cement - ASTM C150 Hydrated Lime - ASTM C207 Masonry Cement - ASTM C91 Mortar Cement - ASTM C1329 Sand – ASTM C144 Additives – ASTM C1384 Pigments – ASTM C979 Water (Potable)
* Typically, based on experience with local materials and conditions, the masonry contractor is an excellent resource for determining the most appropriate and successful mortar materials and proportions.
Cementitious Materials Portland Cement and Hydrated Lime n
Early mortars were hydrated lime and sand. “Hydrated lime contributes to workability, water retentivity, and elasticity. Lime mortars carbonate gradually under the influence of carbon dioxide , a process slowed by cold, wet weather.1”
The invention of Portland cement enabled mortar to develop greater strengths sooner. Originally, Portland was added to lime plaster as the minority constituent. With the demand for stronger and faster reacting mortar, Portland became the majority constituent.
Cementitious Materials Masonry Cements n
Type N Masonry cements were developed by the Portland cement industry prior to WWII. “Masonry cements are proprietary products usually containing portland cement and fines, such as ground limestone or other materials in various proportions, plus additives such as air entraining and water repellency agents.1” Combinations of Type N Masonry cement and Portland cements were included as approved combinations in ASTM C270 for higher strength mortars.
Type S and M Masonry Cements were developed by the Portland cement industry in the 1950s-1960s. The development of a high-strength Masonry cement eliminated the need to mix 2 cementitious materials on the jobsite, making it more convenient and more consistent.
Cementitious Materials Mortar Cements n
Mortar Cements were developed in the late 1980s through the effort of the Masonry Industry Codes Committee. “Mortar cement is a hydraulic cement similar to masonry cement, but the specification for Mortar Cement requires lower air contents and includes a flexural bond strength requirement.1” Mortar cements have flexural bond strengths equivalent to Portland cement and hydrated lime; and, are approved for use in all seismic zones.
Cementitious Materials ASTM C270 Permits All Cementitious Types 5. Requirements â€œ5.1 Unless otherwise stated, a cement/lime mortar, a mortar cement mortar, or a masonry cement mortar is permitted.â€?
Cementitious Materials PCA MASONRY INFORMATION “Selecting and Specifying Mortar and Grout for Unit Masonry” Portland Lime Mortar vs. Mortar Cement Mortar “Mortar cement mortars are used on an equivalent basis as cementlime mortars. The specifier should confirm that mortar types and materials indicated in project specifications are consistent with structural design requirements of the masonry.”
Aggregate for Mortar
Aggregate for Mortar ASTM C144 – Aggregate for Masonry Mortar Property Criteria n Natural or Manufactured Sand n Gradation ranges for particle size n
Provision for sands capable of producing a C270 mortar.
Limits on deleterious substances and organic impurities Soundness limits n
Provision for sands demonstrating 5 year acceptable performance
Step 3 Determine Mortar Specification
ASTM C270 - Two Specifications n
Proportion Specification - based on compliance to proportioning tables.
Property Specification - based on laboratory results of mortar mixture.
When neither are specified, the Proportion Specification shall govern.
Proportion Specification 5.2 Proportion Specification â€” Mortar conforming to the proportion specification shall consist of a mixture of approved materials meeting the proportion requirements in Table 1.
Property Specification 5.3 Property Specificationsâ€” Mortar conformance to the property specifications shall be established by tests of laboratory prepared mortar in accordance with Section 6 and 7.2. Table 2: Laboratory prepared mortar mixed with a quantity of water to produce a flow of 110 Âą 5 %. Note: This quantity of water is not sufficient to produce a mortar with a workable consistency suitable for laying masonry units in the field. This flow better represents the mortar in the wall.
Step 4 Determine Mix Proportions
Section 6. Test Methods 6.1 Proportions of Materials for Test Specimensâ€” Laboratory mixed mortar used for determining conformance to this property specification shall contain construction materials in proportions indicated in project specifications. 6.2 Mixing 6.3 Water Retention 6.4 Air Content 6.5 Compressive Strength NOTE 1â€”When the property specification is used to qualify masonry mortars, the testing agency performing the test methods should be evaluated in accordance with Practice C1093.
Masonry Unit Absorption Masonry unit absorbs moisture from the mortar resulting in a lower W:C ratio.
Step 5 Specify a Quality Assurance Procedure
Quality Assurance 8.1 Compliance to this specification is verified by confirming that the materials used are as specified, meet the requirements as given in Section 2.1, and added to the mixer in the proper proportions. Proportions of materials are verified by: n n n
8.1.1 Implementation and observation …… 8.1.2 Test Method C780 Annex 4, Mortar Aggregate Ratio 8.4 Test Method C1324 Petrographic/Chemical Analysis
*Compliance to either the Proportion Specification or the Property Specification is obtained by the verification of the mix proportions. There is no approved method to accept the mortar by testing for compression in the field.
Quality Assurance 8.1.1 Implementation and observation â€Śâ€Ś
Preconstruction and Construction Evaluation of Mortars for Plain and Reinforced Masonry ASTM C780
ASTM C780 2. Referenced Documents 2.2 The following test methods may be singly or collectively incorporated into the testing to establish mortar composition, â€Ś 2.2.1 Annex A1 - Consistency by Cone Penetration ... 2.2.2 Annex A2 - Consistency Retention ... 2.2.3 Annex A3 - Initial Consistency and Consistency 2.2.4 Annex A4 - Mortar Aggregate Ratio Test Method 2.2.5 Annex A5 - Mortar Water Content Test Method 2.2.6 Annex A6 - Mortar Air Content Test Method 2.2.7 Annex A7 - Compressive Strength of Molded Cylinders â€Ś 2.2.8 Annex A8 - Splitting Tensile Strength ...
ASTM C780 2.2.4 Annex A4 - Mortar Aggregate Ratio Test Method
* Compliance to either the Proportion Specification or the Property Specification is obtained by the verification of the mix proportions.
Quality Assurance There is a 4th method……..
Preblended Dry Mortar Mixes
Mortar Production Systems n
Traditional Field Mixing
Preblended Dry Mortar Bags
Preblended Dry Mortar Silos
Traditional Field Mixing n
Pallets of bagged cement and tons/yards of bulk sand are delivered to the jobsite.
Proportioning is determined by the number of shovels of sand per bag of cement.
Water is added and mixed to the appropriate plasticity.
Preblended Dry Mortar in Bags n
The 80# bag contains a blend of specified cement and dry sand, proportioned to meet the specification.
The bags are added to the masons mixers where water is added and mixed to the appropriate plasticity.
The benefits include: n n n n
Accurate proportioning Less waste and clean up Cleaner jobsite Smaller footprint
Preblended Dry Mortar in Silos n
The silo is delivered and set up on the jobsite. The mason’s mortar mixer is placed under the boot.
The mortar is mixed in the same manner as the preblended bags.
The 3000# bag contains a blend of specified cement and dry sand, proportioned to meet the specification.
ASTM C 1714
ASTM C 1714 n
Produced to meet ASTM C270 criteria n n n
Manufacturing process n n n n
Specified mortar type Same mortar materials criteria Same mix proportioning
Dry materials measured by weight within tolerances Thoroughly blended under QA/QC conditions Traceability of each batch/run Batch records archived
Sampling and Testing n n
Proportion specification – verification of ingredient proportions Property specification – ASTM C270 laboratory testing
Ensuring Mortar Appearance
Factors Affecting Mortar Color Properly mixing the mortar n Correctly placing flashing & weeps n Covering materials & walls as built n Tooling joints properly n Cleaning masonry effectively n Curing n
Properly mixing the mortar 8.1.1 Implementation and observation â€Śâ€Ś
Correctly placing flashing & weeps
Tooled when the mortar is “thumb print hard”.
Too soon will pull a high water content paste to the surface, resulting in a lighter colored joint.
Too late will prevent the paste to be pulled to the surface, resulting in a darker joint.
The moisture content and absorption rate of the unit will affect the rate of moisture loss from the mortar to the unit, impacting the time of tooling.
Timing vs. Moisture A brick prism laid with a single batch of mortar. The top joint was tooled immediately after placement, the remaining mortar joints were tooled at progressively greater time intervals. The only variable was the amount of moisture in the mortar at time of tooling.
Wetter = Lighter
Dryer = Darker
Variable IRA in Units
Variations in the Initial Rate of Absorption at the time of placement will affect the moisture within the brickwork, and could cause mottled mortar joint color.
Cleaning Masonry Commercial cleaning materials should always be used according to the manufacturer's recommendations.
Determine appropriate water pressure, nozzle type, and distance between wall and nozzle.
Weather can affect the final mortar color.
Temperature affect how the mortar cures, causing slight color variations.
Mortar cured under different moisture conditions, can cause differences in joint color.
These differences become less with time as the moisture level stabilizes in the wall.
Moisture Within Mortar Joint
• Avoid making decisions regarding mortar joint color consistency too quickly. Walls should have the opportunity to “mature” through a complete cycle of seasons. • Decisions to stain or replace sections of mortar too quickly will prevent them from matching adjacent sections of mortar later as they mature.
Predicting Mortar Appearance
Sample panels built prior to construction, representative of intended materials and conditions are strongly recommended. Varying the moisture content of several bricks within the panel will demonstrate the range of potential color variation in the mortar joints. Panels should be kept on the jobsite until the completion and acceptance of the brickwork.
This concludes the American Institute of Architects Continuing Education Program.
Thank you for your time!
Published on Oct 23, 2013